Comparative Study of Phase Transformation in ... Comparative Study of Phase Transformation in...
Embed Size (px)
Transcript of Comparative Study of Phase Transformation in ... Comparative Study of Phase Transformation in...
Comparative Study of Phase Transformation in Single-Crystal Germanium during Single and Cyclic Nanoindentation
Koji Kosai ID , Hu Huang ID and Jiwang Yan * ID
Department of Mechanical Engineering, Faculty of Science and Technology, Keio University, Yokohama 2238522, Japan; email@example.com (K.K.); firstname.lastname@example.org (H.H.) * Correspondence: email@example.com; Tel.: +81-45-566-1445
Academic Editor: Ronald W. Armstrong, Stephen M. Walley and Wayne L. Elban Received: 30 September 2017; Accepted: 30 October 2017; Published: 1 November 2017
Abstract: Single-crystal germanium is a semiconductor material which shows complicated phase transformation under high pressure. In this study, new insight into the phase transformation of diamond-cubic germanium (dc-Ge) was attempted by controlled cyclic nanoindentation combined with Raman spectroscopic analysis. Phase transformation from dc-Ge to rhombohedral phase (r8-Ge) was experimentally confirmed for both single and cyclic nanoindentation under high loading/unloading rates. However, compared to single indentation, double cyclic indentation with a low holding load between the cycles caused more frequent phase transformation events. Double cyclic indentation caused more stress in Ge than single indentation and increased the possibility of phase transformation. With increase in the holding load, the number of phase transformation events decreased and finally became less than that under single indentation. This phenomenon was possibly caused by defect nucleation and shear accumulation during the holding process, which were promoted by a high holding load. The defect nucleation suppressed the phase transformation from dc-Ge to r8-Ge, and shear accumulation led to another phase transformation pathway, respectively. A high holding load promoted these two phenomena, and thus decreased the possibility of phase transformation from dc-Ge to r8-Ge.
Keywords: single crystal; germanium; nanoindentation; phase transformation; crystal defect; cyclic load
Pressure-induced formation of various metastable polymorphs takes place in single-crystal germanium (Ge) during diamond anvil cell (DAC) and nanoindentation tests. Previous studies reported that diamond cubic Ge (dc-Ge) transforms to metallic (β-Sn)-Ge at a pressure of ~10 GPa [1–4]. When the pressure releases, this metallic phase transforms to various metastable structures depending on the experimental conditions, such as simple tetragonal phase (st12-Ge) [5–8], rhombohedral phase (r8-Ge) [6,7,9,10], body centered cubic phase (bc8-Ge) [5,6,11], as well as amorphous Ge (a-Ge) and dc-Ge as end phases [8,11]. Another phase of hexagonal diamond Ge (hd-Ge) is also confirmed by compression of a-Ge [9,12,13].
These polymorphs possess very different characteristics from their lowest energy structures, which may open up new applications in future microelectronics and photovoltaics. For this purpose, the complicated phase transformation process of Ge has been widely investigated. For example, in the DAC experiment by Nelmes et al., decompression speed was found to be critical for phase transformation, i.e., slow decompression caused phase transformation to st12-Ge while fast decompression promoted phase transformation to bc8-Ge . Some other studies by nanoindentation on dc-Ge reported more
Crystals 2017, 7, 333; doi:10.3390/cryst7110333 www.mdpi.com/journal/crystals
http://www.mdpi.com/journal/crystals http://www.mdpi.com https://orcid.org/0000-0003-4512-6400 https://orcid.org/0000-0002-3778-4457 https://orcid.org/0000-0002-5155-3604 http://dx.doi.org/10.3390/cryst7110333 http://www.mdpi.com/journal/crystals YANJ テキストボックス Downloaded from Yan Laboratory, Keio University at http://www.yan.mech.keio.ac.jp. Redistribution is subject to copyright licence from the journal publisher.
Crystals 2017, 7, 333 2 of 11
complicated responses against pressure [8,10,11,14]. Slow indentation with a spherical indenter could induce no phase transformation but only plastic deformation by formation of twinning and dislocation slip [8,10,14] which prevented phase transformation by stress release. However, when using a sharp indenter tip, this kind of defect nucleation was suppressed and phase transformations were confirmed . Extremely fast indentation resulted in formation of st12-Ge , and low temperature led to formation of r8-Ge or a-Ge . Investigation of the phase transformation in a-Ge was also performed via indentation [14–17] in which phase transformations can be induced easily compared with dc-Ge because of higher resistance of a-Ge against deformation by slip and twinning. According to the results of indentation on a-Ge, two clear phase transformation pathways via (β-Sn)-Ge have been established . The authors stated that the intermediate (β-Sn)-Ge may transform to two end phases depending on whether the transforming region is constrained or not. Unconstrained (β-Sn)-Ge transforms to dc-Ge with possible trace of st12-Ge while the constrained one undergoes a phase transformation to unstable r8-Ge and finally hd-Ge. They mentioned that both of these two types of phase transformation could occur in the same indent for dc-Ge. The same research team also studied phase transformation behaviors of crystalline Ge by DAC experiment . They classified phase transformations of (β-Sn)-Ge on unloading depending on hydrostaticity. Namely, quasihydrostatic conditions resulted in formation of r8-Ge while the presence of shear led to nucleation of st12-Ge. Their findings were consistent with previously reported phase transformations and helpful to explain the detailed mechanisms [7,14].
Even though the basic phase transformation process of Ge has been classified using a-Ge, it is still important to study and explain dominant phase transformation behaviors of dc-Ge because of the complexity of pressure-induced behaviors . For Si, which has the same crystal structure as Ge, similar pressure-induced phase transformations have been widely reported [1–4,6,18–29], and some new insights into the phase transformation behaviors were further revealed by a multi cyclic nanoindentation method [20–24]. In this current paper, nanoindentation responses of single-crystal Ge under single and double cyclic nanoindentation tests were comparatively investigated. Combined with Raman analysis of residual phases in indents, a dominant phase transformation pathway of dc-Ge under repetitive pressure was established, which may open up new insights into pressure-induced phase transformations of crystalline Ge.
2. Experimental Details
A dc-Ge (111) wafer with thickness of 0.9 mm was used for experiments. Nanoindentation tests were performed on an ENT-1100a nanoindentation instrument (Elionix Inc., Tokyo, Japan) equipped with a Berkovich diamond indenter. In this experiment, single and double cyclic nanoindentation tests were carried out according to the protocol as shown in Figure 1 and the parameters in Table 1. Firstly, the indentation load increased to 50 mN under a given loading rate, held for one second, and then decreased under the same unloading rate as loading rate. For comparison, various loading/unloading rates—10, 25, or 50 mN/s—were used. For the single mode, the indentation load returned to 0 mN and then the test finished, while for the double mode, unloading stopped at a controlled residual load (∆P) and then held for a given load holding time (LHT). As listed in Table 1, ∆P was varied from 0 to 14 mN with LHT of 5 s. Nanoindentation tests with LHT of 20 s were also conducted under ∆P = 2 mN for comparison. After LHT, the second cycle indentation progressed with the same process as single mode from ∆P. For each experimental condition, 20 nanoindentation tests were performed to ensure the reliability of the results.
Residual phases of the all indents were measured by the NRS-3000 Raman micro-spectrometer (JASCO, Tokyo, Japan) with a 532 nm wavelength laser focused to a ~1 µm spot size. To ensure that the residual phases were minimally affected by further phase transformation at room temperature [5,11,13], the measurement of residual phases in indents was performed within three hours after indentation. In previous studies, some specific deformation responses, for example pop-in, pop-out, and elbow have been reported in indentation studies of Si [20–28] and Ge [8,10,11,14–16,23]. In this study, the effects of
Crystals 2017, 7, 333 3 of 11
experimental parameters on these deformation responses were statistically analyzed as well as phase transformation process during both single and cyclic indentation.
Crystals 2017, 7, 333 3 of 10
study, the effects of experimental parameters on these deformation responses were statistically analyzed as well as phase transformation process during both single and cyclic indentation.
Figure 1. Nanoindentation experimental protocols: (a) single mode; (b) double cyclic mode.
Table 1. Experimental parameters for each indentation mode.
Indentation Mode Maximum Load (mN)
Loading/Unloading Rate (mN/s) ∆P (mN) Length of LHT (s)
Single 50 10, 25, 50
Double cyclic 0, 2, 6, 10, 14 5 (or 20 for ∆P = 2 mN)
3. Results and Discussions
3.1. Correlation between Specific Deformation Responses during Nanoindentation Tests and Phase Transformation Behaviors
Figure 2 illustrates typical load-displacement curves obtained under single and double cyclic nanoindentation tests, with shift of the second cycle curves in double cyclic nanoindentation for clarity. For both testing modes, pop-in events marked by arrows in Figure 2 are observed duri